SPONTANEOUS GLASS BREAKAGE
Spontaneous glass breakage is a common phenomenon BINDING OF GLASS IN THE FRAME
where heat-treated glass suddenly breaks without any As a result of strong winds and temperature variations,
apparent reason. This occurrence can be related to glass contracts and expands, therefore, it is recommended
damages during the construction phase, on-site storage, that glass must be set on resilient blocks at the bottom
binding of the glass, thermal stress or internal defects with space for expansion at the sides. If there is no space
within the glass. provided, the glass will bind against the frame resulting in
To identify and minimize the causes of this phenomenon, breakage.
it’s important to consider that only certi ed THERMAL STRESS
manufacturers who meet high standards, by regularly Thermal stress emerges from a di erential expansion
monitoring the production process, can guarantee the within heat-treated glass caused by heating or cooling
quality of its glass, therefore, customers should be aware some areas of the panel. When glass is installed in a
of any glass manipulation during the construction, window, its edges are covered from sunlight by the
storage and installation phase. window frames, therefore, the covered glass edges will be
TECNOGLASS, as an industry leader, shares information cooler than the central area of the glass which is exposed
about the most common reasons that can a ect the glass to the sun.
and result in breakage. The expansion of the central area, due to heating, will
cause the glass to stretch and at the same time, it will be
HOW TO IDENTIFY AND MINIMIZE SPONTANEOUS resisted by the cooler covered edges, which will,
GLASS BREAKAGE consequently, create thermal stress breakage.
DAMAGE DURING THE CONSTRUCTION PHASE FEATURES WHICH INFLUENCE THE DEVELOPMENT OF
When glass is being transported and installed, it’s easy THERMAL STRESS
and likable for the glaziers to nick or chip the glass edges Tensile stress
with di erent kinds of tools. These small nicks or chips Tensile stress develops when the expansion of the central
may not result in instantaneous breakage, but, over a area of the panel is warmer, while the cooler covered
period of time, stress concentrations can develop around edges are trying to resist it. When the expansion of the
the nick, leading to spontaneous breakage. edges becomes su ciently hefty, the tensile stress will
ON-SITE STORAGE exceed a critical point and breakage will form. This is a
To avoid glass breakage on site storage during result of the glass heated non-uniformly, meaning that
construction period, it’s important to identify the places temperature gradients within the glass are exposed to
where the crates - that storage the glass - are going to be temperature di erences.
placed, especially for high performance coated insulating Glass edges and shadows
glass. Due to its heat-re ective nature, the probability of Temperature gradients may occur in glazed windows due
thermal stress breakage increases in these types of glass. to the cool covered edges of the window frames versus
TECNOGLASS recommends not leaving them partially or the heated glass central portion. The framework of the
fully exposed to sunlight to avoid the chances of glass windows usually captures approximately 13 mm of glass
breakage in crates. edge making this area out of reach of sunlight.
Consequently, the glass edge is cooler and temperature
increase is much slower than the central area where it
receives higher heating due to the sun.
TECHNICAL INFORMATION TYPES OF GLASS BREAKAGE
The glass edge in a window may as well presence a shade, Fully - tempered Heat-strengthened
which makes a greater case to thermal stress to occur. Glass Break Glass Break
Shadows are commonly found across glass by balcony
overhangs, eaves, mullions, columns, etc. As the shadow Picture 2. Types of glass breakage.
increases, a superior temperature di erence - higher
tensile stress – is created between the central glass Outdoor shading patterns
exposed to the sun and the shaded glass area, increasing In order to avoid extreme temperature gradients, it’s
the probability of thermal stress and the likelihood of important to consider that shading patterns may vary
glass breakage. seasonally. Tecnoglass recommends minimizing the
project’s location where less than 50% of the glass panel
PROCESS OF THERMAL STRESS BREAKAGE is covered with a shadow as shown in picture 3.
Areas of high stress
(glass tends to contract)
Heated central portion:
(glass tends to expand)
The centre area of the
glass expands while the
edges are under stress
solar radiation High temperature
Picture 1. Process of thermal stress breakage Shading pattern:
Types of glass
Coated and tinted glass are frequently at a higher risk of Picture 3. Outdoor shading pattern.
thermal stress breakage. This may occur because of the
possible temperature imbalance within glass due to solar Indoor shading devices
absorption at the central glass area versus the covered Indoor shading devices may produce temperature
glass edge area. These glass types can be found in gradients on the glass. Picture 4 illustrates how an indoor
TECNOGLASS’ traditional high-performance Low-E device, like blinds, re ects the solar radiation back to the
coatings on tinted glass. glass panel. This reduces the convection and conduction
These glass types require a base glass substrate, on which of the heat apart from the glass, increasing the probability
the coating is applied to be heat-strengthened (HS) or of thermal stress, and in time, breakage.
fully-tempered (FT). For safety glazing applications,
Tecnoglass recommends fully-tempered glass since it’s tecnoglass.com
four times stronger than regular annealed glass of similar
speci cations. Unlike heat-strengthened glass, when the
fully-tempered glass is broken, it breaks in to fairly small,
pebble-like pieces, which reduces the chance of injuries.
solar radiation Solar heat radiation Therefore, TECNOGLASS strongly recommends working
High temperature closely with your glass fabricator and getting a thermal
stress analysis done early in your design process.
Low temperature TECNOGLASS HEAT SOAK TEST
Nickel Sul de (NiS) inclusions
Picture 4. Indoor shading illustration. Nickel sul de is present in the glass as an imperfection
barely visible to the human eye. When a glass is
Heating location and orientation heat-treated in order to obtain fully-tempered glass, NiS
In any residential or commercial project, heating vents inclusions change size as a function of time and
should be carefully placed to ensure that warm air isn’t temperature. When cooled quickly, the NiS particles are
being directed at the glass, which can cause a heat up unable to change completely back to its original form.
and, eventually, breakage. Tecnoglass advises following Over a certain time, NiS will slowly convert to its form but
this recommendation no matter the building’s type or with an increase in volume that can cause breakage.
location. Heat Soak test
INTERNAL DEFECTS WITHIN THE GLASS To avoid this phenomenon, TECNOGLASS uses the Heat
Nickel sul de (NiS) inclusion is a natural occurrence in Soak Test, subjecting tempered glass to extremely
glass, where small particles can still be present during the adverse conditions, therefore, the ones with nickel sul de
fully-tempered and installation process and are inclusions will break in the test.
impossible to see. When tempering a glass containing NiS, If the glasses do not break during the test, TECNOGLASS
the molecule will contract, and during the cooling gives a certi cation to guarantee that the products have
process, it will expand, trying to return to its natural size successfully passed the quality control. This kind of
resulting in glass breakage. breakage is very unusual to happen, but TECNOGLASS can
To avoid the risk of spontaneous breakage in run the test if clients require it to minimize the risk of
fully-tempered glass, TECNOGLASS recommends using spontaneous breakage later in time.
the heat soak test. Upon request, TECNOGLASS will use Heat Soak process
the test, certifying that the glass does not contain any The temperature conditions to which glass is subjected is
nickel sul de and guarantee that there is not any internal between 260°C (500°F) ± 10°C (50°F), this heating process
defect within the glass. lasts approximately 2 hours. Then, the glass enters a
When a glass is heat soaked, the heat converts the nickel maintenance phase for a minimum of 2 hours. Finally, it
sul de inclusion to a high-temperature state and cool it goes to the cooling phase until the temperature of the
right away, resulting in glass breakage or in an optimum glass reaches 70°C (158°F). The whole heat soak cycle lasts
fully-tempered glass. All the above factors can increase or approximately 5 hours and 30 minutes.
decrease the likelihood that a conventional glazed
window will experience thermal stress breakage. T
d a b ct
T glass temperature at any point, °C d ambient temperature
t time, h a heating phase
1 rst glass to reach 250 °C b holding phase
2 last glass to reach 250 °C c cooling phase
Picture 5. Tecnoglass tempered glass heat soak test report, 2011.
Tecnoglass runs this test by EN-14179-1 and EN-14179-2
If you are interested to learn more about how to identify
and minimize spontaneous glass breakage or about our
Heat Soak Test, don’t hesitate to contact us.
The information contained herein is exclusive property of TECNOGLASS, who reserves the right to tecnoglass.com
modify it, including but not limited to the designs and its specications, without notice.
©2019 TECNOGLASS. All rights reserved.